| ||Format||Pages||Price|| |
|6||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$44.00||  ADD TO CART|
Significance and Use
5.1 This practice provides requirements for standardized preparation of sample butt fusions, preparation of specimens from sample butt fusions, and conditioning for testing in accordance with Test Method D638, Test Method D1598, or Test Method D1599. This practice is intended to improve the ability to reliably compare test results from multiple parties.
1.1 This practice provides standardized sample butt fusion preparation, conditioning, and testing conditions for tension testing of specimens prepared from sample butt fusion joints or hydrostatic tests of sample butt fusion joints in accordance with:
1.2 Test Method D1598, constant (sustained) hydraulic pressure testing;
1.3 Test Method D1599, short-term hydraulic pressure testing.
1.4 It is not within the scope of this practice to include plastic materials other than polyethylene or other tests for butt fusions. The exclusion of other plastic materials and other tests does not imply that other plastic materials are suitable or unsuitable for butt fusion, or that the tests cited herein are adequate or inadequate for qualitative characterization and for research and development of butt fusion joints, or that other tests do not have lesser, equal, or greater utility for such purpose.
1.5 The evaluation of test results and the determination of test result evaluation criteria are not within the scope of this practice. This practice is limited to standardized butt fusion test specimens and testing conditions for the comparison of test data from multiple parties.
1.6 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.7 In this standard, text in parentheses, notes in the body of the standard and appendices are informational and non-mandatory. For tables in the body of the standard, table notes are mandatory.
ICS Number Code 23.040.20 (Plastic pipes); 23.040.45 (Plastic fittings)
UNSPSC Code 40170000(Pipe piping and pipe fittings); 13111016(Polyethylene)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM F2928-13, Standard Practice for Specimens and Testing Conditions for Testing Polyethylene (PE) Pipe Butt Fusions Using Tensile and Hydrostatic Test Methods, ASTM International, West Conshohocken, PA, 2013, www.astm.orgBack to Top